Why measure particle size of pharmaceuticals??? Particle size can affect Final formulation: performance, appearance, stability “Processability” of powder (API or excipient). Particle Size Analysis. Microscopy Sieving Sedimentation techniques Optical and electrical sensing zone method
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
Electron microscopy (0.001µ-)
Being able to examine each particle individually has led to microscopy being considered as an absolute measurement of particle size.
Can distinguish aggregates from single particles
When coupled to image analysis computers each field can be examined, and a distribution obtained.
Most severe limitation of optical microscopy is the depth of focus being about 10µm at x100 and only 0.5µm at x1000.
With small particles, diffraction effects increase causing blurring at the edges - determination of particles < 3µm is less and less certain.Microscopy
TEM (Transmission Electron Microscopy) or
SEM (Scanning Electron Microscopy).
TEM and SEM (0.001-5µm)
The length of the line which bisects the particle image. The lines may be drawn in any direction which must be maintained constant for all image measurements.
Feret's diameter (F)
is the distance between two tangents on opposite sides of the particle, parallel to some fixed direction.
Projected area diameter (da or dp)
is the diameter of a circle having the same area as the particle viewed normally to the plane surface on which the particle is at rest in a stable position.
a measured diameter equal to the maximum value of Feret's diameter.
the diameter of a circle having the same circumference as the perimeter of the particle.
a diameter equal to the maximum length of a line parallel to some fixed direction and limited by the contour of the particle.Types of Diameters
Each particle individually examined - detect aggregates, 2D shape, colour, melting point etc.
Permanent record - photograph
Small sample sizes required
Time consuming - high operator fatigue - few particles examined
Very low throughput
No information on 3D shape
Certain amount of subjectivity associated with sizing - operator bias
Particles are individually examined
Visual means to see sub-micron specimens
Particle shape can be measured
Time consuming sample preparation
Materials such as emulsions difficult/impossible to prepare
Low throughput - Not for routine use
Faster and less operator fatigue than manual
No operator bias
Can be very expensive
No human judgement retained e.g. to separate out aggregates, select or reject particles etc. (unlike semi-automatic)
Sieves can be referred to either by their aperture size or by their mesh size (or sieve number).
The mesh size is the number of wires per linear inch.
Approx. size range : 5µm - ~3mm
Standard woven wire sieves
Electroformed micromesh sieves at the lower end or range (< 20µm)
Punch plate sieves at the upper range.Sieving
Easy to perform
Wide size range
Known problems of reproducibility
Wear/damage in use or cleaning
Rod-like particles : overestimate of under-size
Appendix XVII A. Particle Size of PowdersParticle size classification of powders
(Ph. Eur. method 2.9.12, Sieve test)
The degree of fineness of a powder may be expressed by reference to sieves that comply with the specifications for non-analytical sieves (2.1.4).
Where the degree of fineness of powders is determined by sieving, it is defined in relation to the sieve number(s) used either by means of the following terms or, where such terms cannot be used, by expressing the fineness of the powder as a percentage m/m passing the sieve(s) used.
The following terms are used in the description of powders:
Coarse powder: Not less than 95% by mass passes through a number 1400 sieve and not more than 40 % by mass passes through a number 355 sieve.
Moderately fine powder: Not less than 95% by mass passes through a number 355 sieve and not more than 40% by mass passes through a number 180 sieve.
Fine powder: Not less than 95% by mass passes through a number 180 sieve and not more than 40% by mass passes through a number 125 sieve.
Stokes's Law :
Stokes's diameter (dst) is defined as the diameter of the sphere that would settle at the same rate as the particleSedimentation techniques
(1) Incremental : changes with time in the concentration or density of the suspension at known depths are determined. Can be either fixed time or fixed depth techniques.
(2) Cumulative : the rate at which the powder is settling out of suspension is determined. i.e the accumulated particles are measured at a fixed level after all particles between it and the fluid's surface have settled.
Each sample will contain a representative sample of the suspension, with the exception of particles greater than a critical size, all of which will have settled below the level of the sampling point.
The concentration of solid in a sample taken at time t is determined by centrifugation of the sample followed by drying and weighing or simply by drying and weighing.
This concentration expressed as a percentage of the initial concentration gives the percentage (w/w) of particles whose falling velocities are equal to or less than x/t. Substitution in the equation above gives the corresponding Stokes' diameter.Andreasen Pipette
Equipment required can be relatively simple and inexpensive.
Can measure a wide range of sizes with considerable accuracy and reproducibility.
Sedimentation analyses must be carried out at concentrations which are sufficiently low for interactive effects between particles to be negligible so that their terminal falling velocities can be taken as equal to those of isolated particles.
Large particles create turbulence, are slowed and are recorded undersize.
Careful temperature control is necessary to suppress convection currents.
The lower limit of particle size is set by the increasing importance of Brownian motion for progressively smaller particles.
Particle re-aggregation during extended measurements.
Particles have to be completely insoluble in the suspending liquid.
The number and size of particles suspended in an electrolyte is determined by causing them to pass through an orifice an either side of which is immersed an electrode.
The changes in electric impedance (resistance) as particles pass through the orifice generate voltage pulses whose amplitude are proportional to the volumes of the particles.
Volume distributionElectrical sensing zone method – Coulter Counter
Advantage of not requiring medium to be an electrolyteOptical sensing zone method
The angles of diffraction are, in the simplest case inversely related to the particle size.
The particles pass through an expanded and collimated laser beam in front of a lens in whose focal plane is positioned a photosensitive detector consisting of a series of concentric rings.
Distribution of scattered intensity is analysed by computer to yield the particle size distribution.Laser diffraction
Non-intrusive : uses a low power laser beam
Fast : typically <3minutes to take a measurement and analyse.
Precise and wide range - up to 64 size bands can be displayed covering a range of up to 1000,000:1 in size.
Absolute measurement, no calibration is required. The instrument is based on fundamental physical properties.
Simple to use
volume measurement all other outputs are numerical transformations of this basic output form, assuming spherical particles
must be a difference in refractive indices between particles and suspending medium
PCS uses the rate of change of these light fluctuations to determine the size distribution of the particles scattering light.
Comparison of a "snap-shot" of each speckle pattern with another taken at a very short time later (microseconds).
The time dependent change in position of the speckles relates to the change of position of the particles and hence particle size.
The dynamic light signal is sampled and correlated with itself at different time intervals using a digital correlator and associated computer software.
The relationship of the auto-correlation function obtained to time intervals is processed to provide estimates of the particle size distribution.PCS
Nanometre size range
Sample prep critical
Vibration, temperature fluctuations can interfere with analysis
Restricted to solid in liquid or liquid in liquid samples
Need to know R.I. values and viscosity